As a quality-conscious organisation, we make a point of implementing and adhering to stringent and rigorous quality control measures that adhere to international standards throughout the manufacturing process. This enables us to maintain the highest possible quality standards for our products. We source the highest-quality rubber from the market's most reputable vendors. Our rubber floorings are made from recycled tyres.
Keeping our customers' safety in mind, we ensure that each product undergoes quality control procedures prior to being dispatched. These products are not only attractive, but also durable, simple to use, safe, and low maintenance. Additionally, we provide a variety of services to ensure our customers' satisfaction, including customization and timely delivery of products that meet their preferred specifications. We inspect at each stage of production to ensure that our products are defect-free.
Our products are subjected to ASTM and EN standards testing. We recognise the critical fall height and the application of wet pouring surfaces for the safety of children and adults. We specialise in high-quality compounds for epdm rubber granules. Our epdm rubber granules are of the highest quality. The company has established its own laboratory to conduct tests on compounds at various stages of production. We will never make a quality compromise. We uphold our brand's values and equities.
Sun-Flex epdm rubber granules meet ROHS, PAH, migration of certain elements, and new european union norms with REACH parameters.
All technical specifications for Sun-Flex rubber products can be found here. We are committed to producing the highest quality rubber products possible by adhering to all specifications based on our previous experiences. We've designed and engineered the optimal size that's simple to install and manage on a global scale.
|Test Method||Test Value||Tested Laboratory Name|
|ASTM D2859 Pill flammability||Excellent pass||TSI Georgia USA|
|ASTM E303-93 Skid Resistance||Excellent pass||TSI Georgia USA|
|ASTM D2240 Hardness Shore||A 60||TUV Rheinland INDIA|
|ASTM F 150 Ground Electrical Resistance||M ohms 168||TUV Rheinland INDIA|
|DIN 53577 Compression Strength Test Thickness = 42mm||Load= 19950.83 N Compression Strength at 25% deflection = 4.39Mpa||TUV Rheinland INDIA|
|ASTM D573/ASTM D412 Tensile Properties (After Aging at 70oC for 72 hrs) Tensile Strength||MPA 1.01||TUV Rheinland INDIA|
|FMVSS 302 Burning Behaviour Test||6.8 mm/min||TUV Rheinland INDIA|
|ASTM G21:2015||Aspergillus nigerATCC16404 Penicillium pinophilum Hedgcock ATCC 9644 Chaetomium glososum ATCC 6205 Trichoderma virens ATCC 9645 Aureobasidium pullulans ATCC 15233||TUV Rheinland INDIA Result No Growth was Observed on the Specimen|
|ASTM C 423 Sound Absorption Coefficients||0.45 Noise Reduction Coefficient (NRC)||TUV Rheinland INDIA|
|AS/ISO 9239.1-2003 Reaction to Fire Tests for Floorings. Determination of the Burning Behaviour using a Radiant Heat Source||CHF Value 1 Non Directional ≤1.1 kW/m² Smoke Value 1 Non Directional 1869 %.min||Australian Wool Testing Authority Ltd - trading as AWTA Product Testing|
|UV Exposure (150*C)||By chemical Analysis ISO: 4 SBR Blend Rubber No effect||Alekh Plastic Testing Centres|
|RoHS Directive||Pass||TUV NORD INDIA|
|BS EN 71‑3:2019 - Migration of Certain elements||Pass||TUV NORD INDIA|
|PAH (AfPS GS 2019:01 PAK)||Pass||TUV NORD INDIA|
|REACH-219 SVHC EC-1907/2006||Pass||TUV NORD INDIA|
|Test Standards||Test Name||Result||Laboratory|
|BS EN 1177:2008||Critical Fall Height||PASS||SMITHERS RAPRA UK|
|BS 7188:1998+A2:2009||Slip Resistance Ease of Ignition||PASS||SMITHERS RAPRA UK|
|Test Name||Test Method||Test Value||Tested Laboratory Name|
|ABRASION||ASTM D 4060: 2019||Wheel: CS -10
Test Load: 1000g
No. of Cycles: 3000
Before Weight (mg) 28940 After 3000 Cycle Weight 28902.3 Weight Loss (mg) 37.7
|FLAMMABILITY||49 CFR PART 571-302 FMVSS 302: 2019||PASS||SGS|
|DENSITY||ASTM D 792: 2020 (Method – A)||1.096 (g/cm³)||SGS|
|DUROMETER HARDNESS (SHORE A)||ASTM D 2240: 2015||65 (Shore A)||SGS|
|TEAR RESISTANCE||ASTM D 624: 2000 (RA: 2012)||17.30 Tear Strength (KN/m)||SGS|
|HARDNESS (SHORE A)||ASTM D 2240: 2015||65 Hardness (Shore A)||SGS|
|TENSILE STRENGTH||ASTM D 412: 2016||2.44 Tensile Strength (MPa) Type Of Machine Used: CRE Test Speed: 500 mm/min.||SGS|
|COMPRESSION SET||ASTM D 395: 2018, Method – B||87.47 Compression Set (%) Compression: 25% thickness Compression Condition: at 100°C for 72 hours||SGS|
|COMPRESSION DEFORMATION||ISO 815-1: 2019 (Method – A)||84.10 Compression Deformation Set (%) Compression: 25% thickness Compression Condition: at 100°C for 72 hours||SGS|
|Pill Flammability||ASTM D2859||Excellent Pass||TSI GEORGIA USA|
|Skid Resistance||ASTM E303-93||Excellent Pass||TSI GEORGIA USA|
|NIJ 0108.01 Level 3||PASS||TBRL, DRDO INDIA|
Note - Please keep in mind that we can send you all physical soft copies via email if the customer has a genuine need for them.